Designation: G 102 – 89 (Reapproved 1999)
Standard Practice for
Calculation of Corrosion Rates and Related Information from Electrochemical Measurements1 This standard is issued under the ﬁxed designation G 102; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A superscript superscript epsilon (e) indicates an editorial change since the last revision or reapproval.
1. Scope Scope
make make result resultss from from differ different ent studie studiess more more compar comparabl ablee and minimize minimize calculation calculation errors errors that may occur in transfor transforming ming electrochemical results to corrosion rate values.
1.1 This practice practice is intended intended to provide provide guidance in converting the results of electrochemical measurements to rates of uniform corrosion. Calculation methods for converting corrosion current density values to either mass loss rates or average penetr penetrati ation on rates rates are given given for most most engine engineeri ering ng alloys alloys.. In addition, addition, some guideline guideliness for converting converting polarizat polarization ion resisresistance values to corrosion rates are provided.
4. Corrosion Current Current Density 4.1 Corrosion current values values may be obtained from galvanic galvanic cells and polarization measurements, including Tafel extrapolations lations or polarizat polarization ion resistanc resistancee measurem measurements. ents. (See ReferReference Test Method G 5 and Practice G 59 for examples.) The ﬁrst step is to convert the measured or estimated current value to current density. This is accomplished by dividing the total current by the geometric area of the electrode exposed to the solution. It is assumed that the current distributes uniformly across the area used in this calculation. In the case of galvanic couples, the exposed area of the anodic specimen should be used. This calculation may be expressed as follows:
2. Referenced Documents 2.1 ASTM Standards: D 2776 2776 Test Methods for Corrosivity Corrosivity of Water in the Absence of Heat Transfer (Electrical Methods) 2 G 1 Practice Practice for Preparing Preparing,, Cleaning, Cleaning, and Evaluating Evaluating Corrosion Test Specimens 3 G 5 Reference Reference Test Test Method Method for Making Potentiostat Potentiostatic ic and Potentiodynamic Anodic Polarization Measurements 3 G 59 Practice for Conducting Conducting Potentiodynamic Polarization Polarization Resistance Measurements 3
where: icor 5 corrosion current density, µA/cm 2, I cor 5 total anodic current, µA, and A 5 exposed specimen area, cm 2. Othe Otherr unit unitss may may be used used in this this calc calcul ulat atio ion. n. In some some computerized polarization equipment, this calculation is made automatically after the specimen area is programmed into the computer. A sample calculation is given in Appendix X1. 4.2 Equivalent Weight —Equiv —Equivale alent nt weight weight,, EW, EW, may be thought of as the mass of metal in grams that will be oxidized by the passage passage of one Faraday (96 489 6 2 C (amp-sec)) of electric charge.
3. Signiﬁcanc Signiﬁcancee and Use 3.1 Electrochemical corrosion corrosion rate measurements measurements often provide results in terms of electrical current. Although the conversion of these current values into mass loss rates or penetration rates is based on Faraday’s Law, the calculations can be compli complicat cated ed for alloys alloys and metals metals with with elemen elements ts having having multiple valence values. This practice is intended to provide guidance in calculating mass loss and penetration rates for such alloys. Some typical values of equivalent weights for a variety of metals and alloys are provided. 3.2 Electrochemical corrosion corrosion rate measurements may provide results in terms of electrical resistance. The conversion of these results to either mass loss or penetration rates requires additional electrochemical information. Some approaches for estimating this information are given. 3.3 Use of this practice will aid in producing producing more consistent corrosion rate data from electrochemical results. This will
NOTE 1—The value of EW is not dependent on the unit system chosen and so may be considered dimensionless.
For pure elements, the equivalent weight is given by: EW 5
where: W 5 the atomic weight of the element, and n 5 the number of electrons required to oxidize an atom of the the elem elemen entt in the the corr corros osio ion n proc proces ess, s, that that is, is, the the valence of the element. 4.3 For alloys, alloys, the equivalent equivalent weight weight is more complex. complex. It is usually assumed that the process of oxidation is uniform and
This practice is under the jurisdiction of ASTM Committee G01 on Corrosion of Metalsand is the direct responsibility of Subcommittee G01.11 on Electrochemical Measurements in Corrosion Testing. Current Current edition edition approv approved ed Feb. Feb. 24, 1989. 1989. Publish Published ed May 1989. 1989. Original Originally ly published as G 102– 89. Last previous edition G 102– 89 (1994) 1. 2 —See 1990 Annual Book of ASTM Standards , Vol 03.02. Discontinued Discontinued —See 1990 3 Annual Book of ASTM Standards Standards,, Vol 03.02. e
Copyright © ASTM, 100 Barr Harbor Drive, West Conshohocken, PA 19428-2959, United States.
1 COPYRIGHT American Society for Testing and Materials
I cor A
G 102 does not occur selectively to any component of the alloy. If this is not true, then the calculation approach will need to be adjusted to reﬂect the observed mechanism. In addition, some rationale must be adopted for assigning values of n to the elements in the alloy because many elements exhibit more than one valence value. 4.4 To calculate the alloy equivalent weight, the following approach may be used. Consider a unit mass of alloy oxidized. The electron equivalent for 1 g of an alloy, Q is then: Q 5 (
unless a better basis is available. A sample calculation is given in Appendix X2 (1).4 4.5 Valence assignments for elements that exhibit multiple valences can create uncertainty. It is best if an independent technique can be used to establish the proper valence for each alloying element. Sometimes it is possible to analyze the corrosion products and use those results to establish the proper valence. Another approach is to measure or estimate the electrode potential of the corroding surface. Equilibrium diagrams showing regions of stability of various phases as a function of potential and pH may be created from thermodynamic data. These diagrams are known as Potential-pH (Pourbaix) diagrams and have been published by several authors (2, 3). The appropriate diagrams for the various alloying elements can be consulted to estimate the stable valence of each element at the temperature, potential, and pH of the contacting electrolyte that existed during the test.
where: ﬁ 5 the mass fraction of the i th element in the alloy, Wi 5 the atomic weight of the i th element in the alloy, and ni 5 the valence of the i th element of the alloy. Therefore, the alloy equivalent weight, EW , is the reciprocal of this quantity: EW 5
1 niﬁ ( Wi
NOTE 2—Some of the older publications used inaccurate thermodynamic data to construct the diagrams and consequently they are in error.
4.6 Some typical values of EW for a variety of metals and alloys are given in Table 1.
Normally only elements above 1 mass percent in the alloy are included in the calculation. In cases where the actual analysis of an alloy is not available, it is conventional to use the mid-range of the composition speciﬁcation for each element,
4 The boldface numbers in parentheses refer to the list of references at the end of this standard.
TABLE 1 Equivalent Weight Values for a Variety of Metals and Alloys Common Designation
Aluminum Alloys: AA1100A A91100 AA2024 A92024 AA2219 A92219 AA3003 A93003 AA3004 A93004 AA5005 A95005 AA5050 A95050 AA5052 A95052 AA5083 A95083 AA5086 A95086 AA5154 A95154 AA5454 A95454 AA5456 A95456 AA6061 A96061 AA6070 A96070 AA6101 AA7072 AA7075
A96161 A97072 A97075
Copper Alloys: CDA110 C11000 CDA220 C22000 CDA230 C23000 CDA260 C26000 CDA280 C28000 CDA444 C44300 CDA687 C68700 CDA608 C60800 CDA510 C51000 CDA524 C52400
Elements w/Constant Valence Al/3 Al/3, Mg/2 Al/3 Al/3 Al/3, Mg/2 Al/3, Mg/2 Al/3, Mg/2 Al/3, Mg/2 Al/3, Mg/2 Al/3, Mg/2 Al/3, Mg/2 Al/3, Mg/2 Al/3, Mg/2 Al/3, Mg/2 Al/3, Mg/2, Si/4 Al/3 Al/3, Zn/2 Al/3, Zn/2, Mg/2 Al/3, Zn/2, Mg/2 Al/3, Zn/2, Mg/2
Zn/2 Zn/2 Zn/2 Zn/2 Zn/2 Zn/2, Al/3 Al/3
Lowest Variable Valence
Cu/1 Cu/1 Mn/2 Mn/2
Second Equivalent Weight 8.99 9.38 9.51 9.07 9.09 9.01 9.03 9.05 9.09 9.09 9.08 9.06 9.11 9.01 8.98 8.99 9.06 9.58
Third Equivalent Weight
Cu/2 Cu/2 Mn/4 Mn/4
9.32 9.42 9.03 9.06
Mn 7 Mn 7
Fourth Equivalent Weight
Cu/1 Cu/1 Cu/1 Cu/1 Cu/1 Cu/1, Sn/2 Cu/1 Cu/1 Cu/1, Sn/2 Cu/1, Sn/2
63.55 58.07 55.65 49.51 46.44 50.42 48.03 47.114 63.32 63.10
Cu/2 Cu/2 Cu/2 Cu/2 Cu/2 Cu/1, Sn/4 Cu/2 Cu/2 Cu/1, Sn/4 Cu/1, Sn/4
2 COPYRIGHT American Society for Testing and Materials
31.77 31.86 31.91 32.04 32.11 50.00 30.29 27.76 60.11 57.04
C u/2, Sn/4 Cu/2, Sn/4
G 102 TABLE 1 Continued Common Designation
CDA655 C65500 CDA706 C70600 CDA715 C71500 CDA752 C75200 Stainless Steels: 304 S30400 321 S32100 309 S30900 310 S31000 316 S31600 317 S31700 410 S41000 430 S43000 446 S44600 20CB3A N08020
Elements w/Constant Valence
Second Equivalent Weight
Third Equivalent Weight
Si/4 Ni/2 Ni/2 Ni/2, Zn/2
Cu/1 Cu/1 Cu/1 Cu/1
50.21 56.92 46.69 46.38
Cu/2 Cu/2 Cu/2 Cu/2
28.51 31.51 30.98 31.46
Ni/2 Ni/2 Ni/2 Ni/2 Ni/2 Ni/2
Fe/2, Cr/3 Fe/2, Cr/3 Fe/2, Cr/3 Fe/2, Cr/3 Fe/2, Cr/3, Mo/3 Fe/2, Cr/3, Mo/3 Fe/2, Cr/3 Fe/2, Cr/3 Fe/2, Cr/3 Fe/2, Cr/ 3, Mo/3, Cu/1
25.12 25.13 24.62 24.44 25.50 25.26 25.94 25.30 24.22 23.98
Fe/3, Cr/3 Fe/3, Cr/3 Fe/3, Cr/3 Fe/3, Cr/3 Fe/2, Cr/3, Mo/4 Fe/2, Cr/3, Mo/4 Fe/3, Cr/3 Fe/3, Cr/3 Fe/3, Cr/3 Fe/2, Cr/3, Mo/ 4, Cu/1
18.99 19.08 19.24 19.73 25.33 25.03 18.45 18.38 18.28 23.83
Nickel Alloys: 200 400 600 800 825
N02200 N04400 N06600 N08800 N08825
Ni/2 Ni/2 Ni/2 Ni/2
Ni/2 Ni/ 2
G N06007 Ni/2 Carbon Steel: (1) 5 Fe/2, Cr/3, Mo/3, Cu/1, Nb/4, Mn/2 (2) 5 Fe/2, Cr/3, Mo/4, Cu/2, Nb/5, Mn/2 Other Metals: Mg M14142 Mg/2 Mo R03600 Ag P07016 Ta R05210 Ta/5 Sn L13002 Ti R50400 Zn Z19001 Zn/2 Zr R60701 Zr/4 Pb L50045
NI/2 29.36 Ni/3 Cu/1 35.82 Cu/2 Fe/2, Cr/3 26.41 Fe/3, Cr/3 Fe/2, Cr/3 25.10 Fe/3, Cr/3 Fe/2, Cr/3, Mo/3, 25.52 Fe/2, Cr/3, Mo/ Cu/1 4, Cu/1 Mo/3, Fe/2 30.05 Mo/4, Fe/2 Fe/2, Cr/ 3, Mo/3, 26.04 Fe/2, Cr/3, Mo/ W/4 4, W/4 Fe/2, Cr/3, Mo/3, 27.09 Cr/3, Mo/4 W/4 (1) 25.46 (2) Fe/2 27.92 Fe/3 (3) 5 Fe/3, Cr/3, Mo/6, Cu/2, Nb/5, Mn/2
19.57 30.12 25.44 20.76 25.32 27.50 25.12 25.90 22.22 18.62
Fe/3, Cr/6 Fe/3, Cr/6 Fe/3, Cr/6 Fe/3, Cr/6 Fe/3, Cr/6, Mo/6 Fe/3, Cr/3, Mo/6 Fe/3, Cr/6 Fe/3, Cr/6 Fe/3, Cr/6 Fe/3, Cr/3, Mo/ 6, Cu/2
15.72 15.78 15.33 15.36 19.14 19.15 16.28 15.58 14.46 18.88
Fe/3, Cr/6, Mo/6 Fe/3, Cr/6, Mo/6
Fe/3, Cr/6, Mo/6, Cu/2
Fe/3, Cr/6 Fe/3, Cr/6 Fe/3, Cr/3, Mo/ 6, Cu/2 Mo/6, Fe/2 Fe/2, Cr/3, Mo/ 6, W/6 Fe/2, Cr/3, Mo/ 6, W/6 (3)
20.73 16.59 21.70
Fe/3, Cr/6, Mo/6, Cu/2 Mo/6, Fe/3 Fe/3, Cr/6, Mo/6, W/6 Fe/3, Cr/6, Mo/6, W/6 (4)
23.52 23.28 23.63 22.04
23.23 17.88 19.14 17.03
(4) 5 Fe/3, Cr/6, Mo/6, Cu/2, Nb/5, Mn/4
Mo/3 Ag/1 Sn/2 Ti/2
12.15 31.98 107.87 36.19 59.34 23.95 32.68 22.80 103.59
Registered trademark Carpenter Technology. Registered trademark Haynes International. NOTE 1—Alloying elements at concentrations below 1 % by mass were not included in the calculation, for example, they were considered part of the basis metal. NOTE 2—Mid-range values were assumed for concentrations of alloying elements. NOTE 3—Only consistent valence groupings were used. NOTE 4—(Eq 4) was used to make these calculations. B
4.7 Calculation of Corrosion Rate —Faraday’s Law can be used to calculate the corrosion rate, either in terms of penetration rate (CR) or mass loss rate (MR) (4): CR 5 K 1
MR 5 K 2 i cor EW
MR 5 g/m2d, and K 2 5 8.954 3 10−3, g cm2 /µA m2 d (Note 3). NOTE 3— EW is considered dimensionless in these calculations.
Other values for K 1 and K 2 for different unit systems are given in Table 2. 4.8 Errors that may arise from this procedure are discussed below.
where: CR is given in mm/yr, icor in µA/cm2, K 1
4.8.1 Assignment of incorrect valence values may cause serious errors (5).
5 3.27 3 10−3, mm g/µA cm yr (Note 3), 5 density in g/cm 3, (see Practice G 1 for density values
4.8.2 The calculation of penetration or mass loss from electrochemical measurements, as described in this standard, assumes that uniform corrosion is occurring. In cases where non-uniform corrosion processes are occurring, the use of these
for many metals and alloys used in corrosion testing),
3 COPYRIGHT American Society for Testing and Materials
G 102 TABLE 2 Values of Constants for Use in Faraday’s Equation Rate
5 Stern-Geary constant, V. 5.3.2 In cases where one of the reactions is purely diffusion controlled, the Stern-Geary constant may be calculated: B
A Penetration Rate Unit (CR) mpy mm/yrB mm/yrB
Icor Unit 2
µA/cm A/m2B µA/cm2
r Unit 3
g/cm kg/m3B g/cm3
K1 0.1288 327.2 3.27 3 10−3
Units of K1A
mpy g/µA cm mm kg/A m y mm g/µA cm y
A/m2B µA/ cm2 A/m2B
0.8953 0.0895 8.953 3 10−3
Units of K2A g/Ad mg cm2 /µA dm2 d mg m2 /A dm2 d
EW is assumed to be dimensionless. SI unit.
methods may result in a substantial underestimation of the true values. 4.8.3 Alloys that include large quantities of metalloids or oxidized materials may not be able to be treated by the above procedure. 4.8.4 Corrosion rates calculated by the method above where abrasion or erosion is a signiﬁcant contributor to the metal loss process may yield signiﬁcant underestimation of the metal loss rate.
NOTE 4—Electrodes exhibiting stable passivity will behave as if the anodic reaction were diffusion limited, except that the passive current density is not affected by agitation.
5. Polarization Resistance
5.3.5 It is possible to estimate baand bcfrom the deviation from linearity of polarization curves in the 20–50 mV region around the corrosion potential. Several approaches have been proposed based on analyses of electrode kinetic models. See Refs (9-11) for more information. 5.3.6 In cases where the reaction mechanism is known in detail, the Tafel slopes may be estimated from the rate controlling step in the mechanism of the reaction. In general, Tafel slopes are given by (12):
5.1 Polarization resistance values may be approximated from either potentiodynamic measurements near the corrosion potential (see Practice G 59) or stepwise potentiostatic polarization using a single small potential step, D E , usually either 10 mV or − 10 mV, (see Test Method D 2776). Values of 6 5 and 620 mV are also commonly used. In this case, the specimen current, D I , is measured after steady state occurs, and D E/ D I is calculated. Potentiodynamic measurements yield curves of I versus E and the reciprocal of the slope of the curve (dE/dI) at the corrosion potential is measured. In most programmable potentiodynamic polarization equipment, the current is converted to current density automatically and the resulting plot is of i versus E . In this case, the polarization resistance is given by dE/di at the corrosion potential and 5.2 is not applicable. 5.2 It is necessary to multiply the dE/dI or DE/ DI value calculated above by the exposed specimen geometric area to obtain the polarization resistance. This is equivalent to the calculation shown in 4.1 for current density. 5.3 The Stern-Geary constant B must be estimated or calculated to convert polarization resistance values to corrosion current density (6, 8). 5.3.1 Calculate Stern-Geary constants from known Tafel slopes where both cathodic and anodic reactions are activation controlled, that is, there are distinct linear regions near the corrosion potential on an E log i plot: B 5
ba bc 2.303 ~ba 1 bc!
where: K 5 a constant, R 5 the perfect gas constant, T 5 the absolute temperature, n 5 the number of electrons involved in the reaction step, and F 5 Faraday’s constant. RT At 25°C, ( ) is 59.2 mV/decade. For simple one 2.303 F electron reactions, K is usually found to be 2.0. 5.3.7 In cases where the Tafel slopes cannot be obtained from any of the methods described above, it may be necessary to determine the Stern-Geary constant experimentally by measuring mass loss and polarization resistance values. 5.4 The corrosion current density may be calculated from the polarization resistance and the Stern-Geary constant as follows:
where: ba 5 slope of the anodic Tafel reaction, when plotted on base 10 logarithmic paper in V/decade, bc 5 slope of the cathodic Tafel reaction when plotted on base 10 logarithmic paper in V/decade, and
B R p
The corrosion rate may then be calculated from the corrosion current, as described in Section 4. A sample calculation is given in Appendix X5. 4
COPYRIGHT American Society for Testing and Materials
where: b 5 the activation controlled Tafel slope in V/decade. 5.3.3 It should be noted in this case that the corrosion current density will be equal to the diffusion limited current density. A sample calculation is given in Appendix X4. 5.3.4 Cases where both activation and diffusion effects are similar in magnitude are known as mixed control. The reaction under mixed control will have an apparently larger b value than predicted for an activation control, and a plot of E versus log I will tend to curve to an asymptote parallel to the potential axis. The estimation of a B value for situations involving mixed control requires more information in general and is beyond the scope of this standard. In general, Eq 7 and Eq 8 may be used, and the corrosion rate calculated by these two approximations may be used as lower and upper limits of the true rate.
B Mass Loss Rate Unit g/m2dB mg/dm2d (mdd) mg/dm2d (mdd)
G 102 5.5 There are several sources of errors in polarization resistance measurements:
cathodic processes, c 5 the electrode capacitance, and dV/dt 5 the scan rate.
5.5.1 Solution resistivity effects increase the apparent polarization resistance, whether measured by the potentiostatic or potentiodynamic methods (13). The effect of solution resistance is a function of the cell geometry, but the following expression may be used to approximate its magnitude. R p 5 Ra 2 rl
The capacitance charging effect will cause the calculated polarization resistance to be in error. Generally, this error is small with modest scan rates (14). 5.5.3 Corroding electrodes may be the site for other electrochemical reactions. In cases where the corrosion potential is within 50 to 100 mV of the reversible potential of the corroding electrode, the electrochemical reactions will occur simultaneously on the electrode surface. This will cause either the anodic or cathodic b value to appear smaller than the corrosion reaction above. Consequently, the Stern-Geary constant B will be inﬂated and the predicted corrosion current will be overestimated (15). In this case, the concentration of the corroding electrode ions is generally of the same magnitude or higher than other ions participating in the corrosion process in the electrolyte surrounding the electrode. Other redox couples that do not necessarily participate in the corrosion reaction may have similar effects. This is especially true for metals exhibiting passive behavior.
where: Ra 5 the apparent polarization resistance, ohm cm 2, r 5 the electrolyte resistivity in ohm cm, l 5 the distance between the specimen electrode and the Luggin probe tip, or the reference electrode in cm, and R p 5 the true polarization resistance in ohm cm 2. Signiﬁcant solution resistivity effects cause the corrosion rate to be underestimated. A sample calculation is given in Appendix X6. 5.5.2 Potentiodynamic techniques introduce an additional error from capacitative charging effects. In this case, the magnitude of the error is proportional to scan rate. The error is illustrated by (Eq 12): I total 5 I f 1 c
S D dV dt
5 the Faradaic current associated with anodic and
where: I total 5 the cell current,
6.1 corrosion current; corrosion rate; electrochemical; equivalent weight; polarization resistance; Tafel slopes
APPENDIXES (Nonmandatory Information) X1. SAMPLE CALCULATION—CORROSION CURRENT DENSITY
X1.2 Calculation— See (Eq 1) in text:
X1.1.1 Corrosion Current —27.0 µA. X1.1.2 Specimen Size—round anode area exposed. X1.1.3 Diameter —1.30 cm.
27.0 5 20.3 µA /cm2 1.32
X2. SAMPLE CALCULATION—ALLOY EQUIVALENT WEIGHT
X188.8.131.52 Iron 5 100 − 31.5 5 68.5 %. X2.2.2 Valence values from Ref (2).
X2.1 Data: X2.1.1 Alloy—UNS S31600, actual composition not available. X2.1.2 Corrosion Potential —300 mV versus SCE 1N sulfuric acid.
Chromium—+3 Nickel—+2 Molybdenum—+3 Iron—+2
X2.3 Calculations— For simplicity, assume 100 g of alloy dissolved. Therefore, the gram equivalents of the dissolved components are given by (Eq 3).
X2.2 Assumptions: X2.2.1 Composition: X184.108.40.206 Chromium16–18 %—mid range 17 %. X220.127.116.11 Nickel—10–14 %—mid range 12 %. X18.104.22.168 Molybdenum—2–3 %—mid range 2.5 %. X22.214.171.124 Iron—Balance (ignore minor elements). 17 1 12 1 2.5 5 31.5
5 0.981 1 0.409 1 0.078 1 2.453 5 3.921 g equivalents
The alloy equivalent weight is therefore
5 COPYRIGHT American Society for Testing and Materials
17 12 2.5 68.5 331 321 331 32 51.996 58.71 95.94 55.847
⁄ 3.921 5 25.50.
G 102 X3. SAMPLE CALCULATION FOR CORROSION RATE FROM CORROSION CURRENT
X3.1 Data and requirements—See X1 and X2.
X3.2 Calculations—See (Eq 5). K 1 5 3.27 3 1023
X3.1.1 Corrosion rate in mm/yr. 3
X3.1.2 Density 8.02 g/cm .
3.27 3 1023 3 20.3 3 25.50 5 0.211 mm/yr 8.02
X4. SAMPLE CALCULATION FOR STERN-GEARY CONSTANT
X4.1 Case 1 Data—Tafel slopes polarization diagram, ba 5 58.2 mV/decade, and
bc 5 114.3 mV/decade.
X4.3 Case 2— Cathodic reaction is diffusion controlled ba 5 58.2 mV/decade
X4.4 Calculation— (Eq 8):
X4.2 Calculation in accordance with (Eq 7).
58.2 3 114.3 5 16.74 mV or 0.01674 V (X4.2) B 5 2.303 ~58.2 1 114.3!
58.2 5 25.31 mV 2.303
X5. SAMPLE CALCULATION—CORROSION CURRENT FROM POLARIZATION RESISTANCE DATA
X5.1 Data—Polarization: 10 mV from corrosion potential.
X5.1.1 Current measured —17.1 µA. X5.1.2 Specimen Size—14.2 mm diameter masked circular area.
5 10.80 µA /cm 2
X5.2.2 Polarization resistance calculation: Rp 5
X5.1.3 Tafel slope values given in X4.
10 mV Ep 5 5 926 ohm cm2 i 10.80 µA /cm 2
X5.2.3 Corrosion current—(Eq 10)
X5.2.1 Current density (see X4):
25.31 mV B 5 5 27.33 µA /cm2 Rp 926 ohm cm 2
X6. SAMPLE CALCULATION—SOLUTION RESISTIVITY EFFECTS Rp 5 Ra 2 r1
Rp 5 9926 2 0.5 3 4000
X6.1.1 Solution Resistivity —4000 ohm cm. X6.1.2 Distance Between Luggin Tip and Specimen—5 mm. X6.1.3 Measured Polarization Resistance —9926 ohm cm2.
Rp 5 9926 2 2000 5 7926 ohm cm 2
NOTE X6.1—The solution resistivity effect causes the corrosion rate to be underestimated by about 25 % in this case.
X6.2 Calculation from (Eq 11):
6 COPYRIGHT American Society for Testing and Materials
G 102 REFERENCES (1) Dean, S. W., Materials Performance, Vol 26, 1987, pp. 51–52. (2) Pourbaix, M., “Atlas of Electrochemical Equilibrium in Aqueous Solutions,” National Association of Corrosion Engineers, Houston, TX, 1974. (3) Silverman, D. C., Corrosion, Vol 37, 1981, pp. 546–548. (4) Dean, S. W., Jr., W. D. France, Jr., and S. J. Ketcham, “Electrochemical Methods,” Handbook on Corrosion Testing and Evaluation, W. H. Ailor, Ed., John Wiley, New York, 1971, pp. 173–174. (5) Dean, S. W., Jr., “Electrochemical Methods of Corrosion Testing,” Electrochemical Techniques for Corrosion, R. Baboian, Ed., National Association of Corrosion Engineers, Houston, TX, 1977, pp. 52–53. (6) Stern, M. and Roth, R. M., Journal of the Electrochemical Society, Vol 105, 1957, p. 390. (7) Stern, M., Corrosion, Vol 14, 1958, p. 440t. (8) Mansfeld, F., “The Polarization Resistance Technique for Measuring Corrosion Currents,” Corrosion Science and Technology, Plenum Press, New York, Vol IV, 1976, p. 163. (9) Barnartt, S., Electrochemical Nature of Corrosion, Electrochemical
Techniques for Corrosion, R. Baboian, Ed., National Association of Corrosion Engineers, Houston, TX, pp. 1–10, 1977. (10) Oldham, K. B. and Mansfeld, F., “Corrosion Rates from Polarization Curves-A New Method,” Corrosion Science, Vol 13, No. 70, p. 813 (1973). (11) Mansfeld, F.,“ Tafel Slopes and Corrosion Rates from Polarization Resistance Measurements,” Corrosion, Vol 29, p. 10 (1972). (12) Glasstone, S., Laidler, K. J., and Eyring, H., “The Theory of Rate Processes,” McGraw Hill, New York, 1941, pp. 552–599. (13) Mansfeld, F., “The Effect of Uncompensated Resistance on True Scan Rate in Potentiodynamic Experiments,” Corrosion, Vol 38, No. 10, pp. 556–559 (1982). (14) Mansfeld, F., and Kendig, M., “Concerning the Choice of Scan Rate in Polarization Measurements,” Corrosion, Vol 37, No. 9, pp. 545–546 (1981). (15) Mansfeld, F., and Oldham, K. L., “A Modiﬁcation of the Stern-Geary Linear Polarization Equation,” Corrosion Science, 1971, Vol 11, pp. 787–796.
The American Society for Testing and Materials takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, 100 Barr Harbor Drive, West Conshohocken, PA 19428. This standard is copyrighted by ASTM, 100 Barr Harbor Drive, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or [email protected]
(e-mail); or through the ASTM website (http://www.astm.org).
7 COPYRIGHT American Society for Testing and Materials